Dr. J. A. Brinell invented the Brinell test in Sweden in 1900. The oldest of the hardness test
methods in common use today, the Brinell test is frequently used to determine the hardness of
forgings and castings that have a grain structure too course for Rockwell or Vickers testing.
Therefore, Brinell tests are frequently done on large parts. By varying the test force and ball
size, nearly all metals can be tested using a Brinell test. Brinell values are considered test
force independent as long as the ball size/test force relationship is the same.
In the USA, Brinell testing is typically done on iron and steel castings using a 3000Kg test
force and a 10mm diameter carbide ball. Aluminum and other softer alloys are frequently tested
using a 500Kg test force and a 10 or 5mm carbide ball. Therefore the typical range of Brinell
testing in this country is 500 to 3000kg with 5 or 10mm carbide balls. In Europe Brinell testing
is done using a much wider range of forces and ball sizes. It's common in Europe to perform Brinell
tests on small parts using a 1mm carbide ball and a test force as low as 1kg. These low load tests
are commonly referred to as baby Brinell tests.
Brinell Test methods are defined in the following standards:
Brinell Test Method
All Brinell tests use a carbide ball indenter. The test procedure is as follows:
- The indenter is pressed into the sample by an accurately controlled test force.
- The force is maintained for a specific dwell time, normally 10 - 15 seconds.
- After the dwell time is complete, the indenter is removed leaving a round indent in the sample.
- The size of the indent is determined optically by measuring two diagonals of the round indent
using either a portable microscope or one that is integrated with the load application device.
- The Brinell hardness number is a function of the test force divided by the curved surface
area of the indent. The indentation is considered to be spherical with a radius equal to half
the diameter of the ball. The average of the two diagonals is used in the following formula
to calculate the Brinell hardness.
The Brinell number, which normally ranges from HB 50 to HB 750 for metals, will increase as
the sample gets harder. Tables are available to make the calculation simple. A typical Brinell
hardness is specified as follows:
Where 356 is the calculated hardness and the W indicates that a carbide ball was used. Note- Previous standards allowed a
steel ball and had an S designation. Steel balls are no longer allowed.
Because of the wide test force range the Brinell test can be used on almost any metallic material.
The part size is only limited by the testing instrument's capacity.
- One scale covers the entire hardness range, although comparable results can only be obtained if
the ball size and test force relationship is the same.
- A wide range of test forces and ball sizes to suit every application.
- Nondestructive, sample can normally be reused.
- The main drawback of the Brinell test is the need to optically measure the indent size.
This requires that the test point be finished well enough to make an accurate measurement.
- Slow. Testing can take 30 seconds not counting the sample preparation time.